Interested in publishing with us ? Contact book

The airway starts at the anterior nasal vestibule and ends at the lung parenchyma. This includes the nasal cavity, nasopharynx, oral cavity, oropharynx, larynx, hypopharynx, trachea, and bronchi. When evaluating a child with noisy breathing, it is important to assess the airway in a systematic manner. A thorough history is important. This includes assessment of the severity or progression of symptoms, and whether the symptoms are worse with feeding or increased exertion. The severity determines the urgency of complete evaluation. Apparent life-threatening events (ALTE) warrant prompt multidisciplinary evaluation (McMurray, 1997). Inspiratory stridor generally originates from the larynx, while expiratory stridor from the trachea or bronchi. Stridor that is biphasic (both inspiratory and expiratory) typically indicates a fixed obstructive lesion is present. Depending on symptomatology, the addition of endoscopic evaluation of the airway to the basic physical examination can be extremely beneficial. A definitive diagnosis is critical to proper treatment intervention.


Introduction
This chapter will review recent progress in the use of atomic layer deposition (ALD) to prepare noble metal nanoparticle catalysts in which the nanoparticle size, composition, and local environment can be tailored on the atomic scale to tune the reactivity, selectivity, and thermal stability of the catalysts.ALD is a thin film growth technique that uses alternating cycles of self-limiting chemical reactions between gaseous precursors and a solid surface to deposit material in an atomic layer-by-layer fashion 1 .By combining ALD processes for metal oxides, noble metals, and other materials relevant to catalysis, it is possible to engineer nanostructured catalysts with unique properties by depositing a sequence of discrete layers or particles which each perform a specific function.Although the idea of using ALD to prepare catalysts is not new 2 , recent advances in ALD technology, coupled with innovative ideas for nanofabrication, have rekindled this field and now offer potential solutions to long-standing problems in catalyst synthesis.
We begin with a brief introduction to ALD.A broad variety of materials can be deposited by ALD using alternating exposures of two chemicals.For example, aluminum oxide (Al 2 O 3 ) ALD uses sequential exposures to trimethyl aluminum (TMA) and H 2 O as illustrated in Fig. 1 3 .In reaction A, the substrate to be coated is exposed to TMA vapor which reacts with surface hydroxyl groups (OH) to form new O-Al linkages and liberate methane (CH 4 ) into the gas phase.This reaction proceeds until all of the OH groups are consumed at which point the reaction terminates because the TMA is inert towards the methyl-terminated surface.In reaction B, H 2 O vapor is introduced which reacts with the surface methyls producing CH 4 gas and again forming new Al-O linkages.Reaction B stops when all of the methyl groups are gone because the H 2 O does not react with surface hydroxyls.The net result of one A/B cycle is to deposit a monolayer of Al 2 O 3 on the surface and to regenerate the original starting surface so that the process can be repeated.
ALD reactors typically incorporate a chamber heated to ~100-400°C containing the substrate to be coated 4 .A constant stream of inert gas such as N 2 flows through the chamber at a pressure of ~0.1-10 Torr.The precursor vapors are injected into the carrier gas using pulsed valves and transported to the substrate where they react, and any excess precursor and byproduct gases are swept away.Desirable characteristics for ALD precursors include high volatility, good thermal stability at the ALD growth temperatures, and high reactivity with the other compound used for the film growth.A purge period is introduced between each precursor dose to prevent mixing of the chemicals which would cause non self-limited growth.Each ALD cycle can last seconds to hours depending on factors such as the reactivity of the precursors and the surface area and porosity of the substrate.ALD research and process development are greatly facilitated using in-situ measurements.For instance, an in-situ quartz crystal microbalance (QCM) with sub-monolayer sensitivity and 10-20 Hz update rate, is a valuable tool for monitoring film growth in real time, and can also provide details for understanding the ALD surface chemistry.Similarly, an in situ quadrupole mass spectrometer (QMS) installed in the reactor can help to understand the growth mechanism by identifying the gas phase products of the ALD surface reactions.One of the hallmarks of an ALD process is that the reactions saturate after a certain minimum exposure, after which additional precursor flux does not deposit more material.For instance, Fig. 2a shows that the Al 2 O 3 ALD saturates at 1.2 Å/cycle following a TMA exposure of ~0.05 Torr s.A natural consequence of this self-limiting behavior is that the film thickness increases by a fixed amount with each A/B cycle.This behavior is displayed in Fig. 2b where the ALD Al 2 O 3 thickness was measured by ellipsometry over a wide range of A/B cycles and the growth is exceptionally linear 5 .A second consequence of the selfterminating surface chemistry is that the precursor molecules can diffuse into narrow pores until they encounter an empty site, and in this way nanoporous materials can be coated with great uniformity.This capability is extremely useful for catalyst synthesis 6 .
Figure 2b demonstrates that the Al 2 O 3 ALD growth rate does not change with the number of cycles, and in particular the earliest cycles deposit virtually the same amount of Al 2 O 3 as the later cycles.This behavior is typical of most ALD metal oxides and results from the prompt nucleation or initiation of metal oxide ALD on most surfaces (due to the ubiquity of OH groups), and usually generates very uniform, continuous films.In contrast, the ALD of noble metals such as palladium often shows a long incubation period on oxide surfaces 7 .This nucleation delay stems from the difficulty in removing the ligands from the noble metal precursor bound to an oxide surface.This poor nucleation, coupled with the natural tendency for noble metal atoms to diffuse and agglomerate, results in the formation of discrete metal islands which grow with increasing numbers of ALD cycles until finally converging to form a continuous film.Although this tendency is undesirable for microelectronics applications, it is ideal for preparing catalytic nanoparticles which must be highly dispersed and of nanometer size.Smaller nanoparticles are typically more active on a per-atom basis because the surface area to volume ratio increases with decreasing thickness.Moreover, the lower radius of curvature for smaller nanoparticles produces a larger fraction of under-coordinated surface atoms, which often have the highest catalytic activity.For these reasons, the following sections will highlight efforts to control the nanoparticle size, and in particular to achieve ultra-small (<1nm) noble metal nanoparticles.In addition to depositing simple binary compounds such as Al 2 O 3 and elements such as Pd, ALD can also synthesize ternary and more complex compounds such as ZnAl 2 O 4 8 , as well as mixed metals such as Pt-Ir 9 .The ALD of mixed materials is accomplished by alternating between the binary reaction sequences of the individual components in the mixture, and the composition is controlled by adjusting the ratio of ALD cycles for the different components.The ability to control the composition of a metal oxide support layer allows properties such as the surface acidity to be adjusted in a manner analogous to the Al/Si ratio in zeolites, and mixed-metal nanoparticles such as Pt-Ru often exhibit superior catalytic properties.
The capability to produce both thin, continuous layers as well as discrete nanoparticles makes it possible to engineer an "ideal catalyst" using a sequence of ALD processes as illustrated in Fig. 3. Starting from a substrate with the desired porosity, surface area, and nanostructure, the support layer is first applied by ALD in the form of a physically thin but chemically thick layer (~1 nm).Next, catalytic nanoparticles are deposited by ALD on top of the support layer with the desired size, composition, dispersion, and nanostructure.A final ALD process can be used to stabilize the nanoparticles against sintering, or to modify their catalytic behavior.The following sections will provide examples for all of the steps in this synthesis scheme.In particular, we will describe ALD of the noble metals Pt, Pd, and Ir, and the mixed-noble metals Pt-Ir, Pt-Ru, and Pt-Pd.We will show the effects of different ALD support layers (Al 2 O 3 , TiO 2 , ZrO 2 , and ZnO) as well as the influence of ALD over-layers on the stability and reactivity of catalytic nanoparticles.

Palladium ALD
Palladium (Pd) is a common metal for heterogeneous catalysis with applications in methanol partial oxidation and the water-gas shift reaction.Palladium ALD can be accomplished using Pd(II) hexafluoroacetylacetonate (Pd(hfac) 2 ) which has a relatively high vapor pressure compared to other β-diketonate derivatives of Pd. 10 Senkevich et al. demonstrated Pd ALD at 80 °C on Ir metal surfaces, where atomic hydrogen, formed from the dissociation of H 2 on the Ir surface, served as the reducing reagent. 11To increase the substrate generality, Ten Eyck et al. used a remote hydrogen plasma for Pd ALD on Ir, W, and Si surfaces. 12However, plasmas are not well suited to catalyst synthesis because they require line-of-site between the plasma and the substrate surface which is impractical for nanoporous catalyst templates.The lack of a suitable reducing reagent for Pd ALD on porous oxide surfaces has limited the development of ALD Pd catalysts.This problem was solved by using formalin as the reducing reagent. 7Pd ALD was investigated using amorphous ALD Al 2 O 3 as the support material.The reaction mechanism during the first Pd ALD cycle was suggested to be:

Control of ALD Pd particle size
In many heterogeneous and electro-catalytic reactions, particle size plays a major role in determining catalyst performance. 15Therefore, a synthesis method which can precisely tune the size of noble metal nanoparticles while maintaining a narrow size distribution can improve the catalytic performance significantly.ALD provides fine control over noble metal nanoparticle size.For instance, the size of Pd nanoparticles on an Al 2 O 3 support was found to vary linearly between 1.1 (± 0.5) nm and 2.9 (± 0.9) nm as the number of Pd ALD cycles was increased from 1 to 25. 14a The size of noble metal nanoparticles often depends on the metal loading since the nanoparticles form through diffusion which is influenced by the inter-particle spacing.
Clearly the Pd loading can be controlled by the number of ALD Pd cycles, but the selflimiting and site-selective nature of ALD provides additional means for controlling the loading.Equation 1implies that the density of surface hydroxyls dictates the number of adsorbed Pd(hfac) 2 precursor molecules during Pd ALD.Therefore, decreasing the surface hydroxyl density should reduce the Pd loading.In agreement with this idea, when the hydroxyl density on an ALD Al 2 O 3 surface was reduced prior to the Pd ALD through thermal treatment, reaction with alcohols to form surface alkoxides, or reaction with TMA, the Pd loading decreased 16 .
Temperature can also affect nanoparticle size in ALD.In situ QCM measurements demonstrated that Pd(hfac) 2 chemisorption on oxide surfaces can occur at temperatures as low as 80°C, far below the minimum temperature of 200°C required to strip the remaining hfac ligands using HCOH .14a, 17 This finding suggested that one route to smaller Pd nanoparticles is to chemisorb the Pd(hfac) 2 at lower temperatures to reduce agglomeration.Indeed, low-temperature deposition of Pd(hfac) 2 yielded a particle size of 0.8±0.2nm, significantly below the 1.4±0.4nm size obtained using the standard 200°C Pd(hfac) 2 adsorption (Fig. 5). 16g. 5. Scanning transmission electron microscopy (STEM) image (a) and corresponding particle size distribution (b) of ALD Pd sample prepared using Pd(hfac) 2 at 100°C, followed by 2-cycle ALD Al 2 O 3 to stabilize the Pd(hfac) 2 species before removing the hfac ligands at 200°C using HCOH. 16e unique advantage of ALD is the capability to tune the metal loading without affecting the particle size.For instance, when an ethanol exposure was used to remove a fraction of the Al 2 O 3 surface hydroxyls by conversion to ethoxide species prior to a lowtemperature Pd(hfac) 2 exposure, the Pd loading dropped by 36%, but the Pd particle size was unchanged. 16In contrast, the Pd loading was found to increase substantially when the conventional Pd(hfac) 2 /HCOH reaction scheme was replaced with a novel Pd(hfac) 2 /TMA/H 2 O sequence for Pd ALD.In this case, the Al 2 O 3 that formed during the interposed TMA/H 2 O exposures continuously provided new nucleation sites for Pd(hfac) 2 chemisorption.Simultaneously, the TMA acted as a reducing agent to remove the hfac ligands.In this way the Pd metal loading from 15 Pd(hfac) 2 exposures increased from 0.7 % to 6.6 % using this novel pulsing sequence while maintaining a Pd nanoparticle size of only ~1 nm. 17

Activity of ALD Pd catalysts
The catalytic activity of ALD Pd nanoparticles was evaluated using the methanol decomposition reaction.The low-temperature decomposition of methanol to form carbon monoxide and hydrogen may provide a valuable source of hydrogen for transportation fuel, 18 and Pd is one of the most active species for catalyzing this process.It is generally believed that smaller Pd particles are more active for methanol decomposition. 19In keeping with this trend, Fig. 6 shows that at the same space velocity (mol of methanol per gram of Pd), the activities of the ALD Pd catalysts increase in the sequence: Pd (2.2 nm) < Pd (1.4 nm) < Pd (0.8 nm).It is worth noting that the hydrogen production rate of the 1.4 nm ALD Pd catalyst at a space velocity of 120 000 mL/h/g-cat was significantly higher than some of the most active Pd-based catalysts reported for this reaction which is likely due to the highly uniform dispersion and small particle size.

Support effects for ALD Pd catalysts
The catalytic behavior of noble metal nanoparticles can be greatly influenced by the underlying support material.For instance, cationic Pd species (most likely Pd + ) formed through the strong metal-support interaction are sometimes invoked to explain the higher activities of smaller Pd particles supported on CeO 2 or ZrO 2 . 20However, support effects are difficult to isolate using traditional catalyst synthesis methods.These methods rely on bulk supports which often have different physical properties such as surface area, pore size distribution, or particle size that can also affect performance.In contrast, ALD can be used to prepare the support as a thin (~1 nm), conformal layer on a template (Fig. 3).In this way, the same template can be used for a variety of ALD support layers allowing the composition to be varied while keeping the physical structure constant.ALD Pd nanoparticle catalysts were prepared on ALD Al 2 O 3 , ZrO 2 , and TiO 2 layers on high surface area silica gel templates.The Pd loading was found to vary somewhat with the support layer (1.69% on Al 2 O 3 , 0.82% on ZrO 2 , and 1.17% on TiO 2 ) and this probably reflects the different reactivity of the Pd(hfac) 2 precursor on these different surfaces.The relative rates of the three catalysts were evaluated for the methanol decomposition reaction, and the absolute rates were divided by the catalyst loading.The relative rates were found to increase as: Al 2 O 3 < TiO 2 < ZrO 2 as shown in Fig.
6 21 .On a per-atom basis, the ALD Pd is 7x more active on the ALD ZrO 2 support compared to the ALD Al 2 O 3 support.Fig. 7. Influence of metal oxide support on relative rate of methanol decomposition for ALD Pd catalysts.

Platinum ALD
Platinum (Pt) nanoparticles were first used as industrial catalysts by Vladimir Haensel at UOP in the 1940s 22 .Since then, Pt nanoparticles have become one of the predominant industrial precious metal catalysts and have received significant academic and industrial attention because of their unique catalytic properties.Supported Pt nanoparticles in the range of sub-nm to a few nm are effective for oxidative dehydrogenation of propane 23 , water-gas shift reaction 24 , fuel cells 25 , direct conversion of methane 26 , bio-mass reforming 27 , and emission control 28 .The high market price of platinum and high activity of under-coordinated surface Pt atoms have motivated efforts to synthesize small Pt nanoparticles with a narrow size distribution using conventional preparation methods such as wet impregnation 29 and colloidal chemistry 30 .In light of the results presented above for Pd, ALD is a promising technique to prepare monodispersed Pt nanoparticles on high surface area supports with precise size control.
Pt ALD is typically conducted using alternating exposures of (trimethyl) methylcyclopentadienyl platinum (IV) (MeCpPtMe 3 ) and oxygen at 300 °C with dose and purge times of several seconds required to coat planar surfaces.
In reaction 3, MeCpPtMe 3 reacts with oxygen adsorbed on the Pt surface from the preceding O 2 exposure.In reaction 4, O 2 serves to combust the remaining ligands on the adsorbed precursor, and some oxygen remains adsorbed on the surface.Pt ALD in the steady state regime is facilitated by the dissociation of O 2 on Pt to produce the necessary O* species.In contrast, we expect that Pt nucleation on oxide surfaces should be hindered because most oxides are not capable of dissociating O 2 at these temperatures.

Pt on SrTiO 3
To study Pt nucleation and growth on a catalytically relevant metal oxide surface, Bedzyk and coworkers prepared Pt nanoparticles on SrTiO 3 (001) single crystals 32 and high surface area SrTiO 3 nanocubes 33 .Contrary to expectations, the Pt growth during the nucleation period on SrTiO 3 (001) was ~2x higher than in the steady-state regime (Fig. 8).The higher initial growth was attributed to a greater density of reactive sites on SrTiO 3 compared to Pt.In contrast to the Pd study which used relatively short exposure times and showed a lower initial growth (Fig. 4), the Pt nucleation in Fig. 8 used much larger precursor exposures that were sufficient to saturate the surface reactions despite a lower reaction rate.Atomic force microscopy and scanning electron microcopy (SEM) revealed that the Pt nucleation occurred by island coalescence on the SrTiO 3 (001) surface, and the diameter of the Pt nanoparticles increased linearly with Pt ALD cycles before achieving film closure at ~40 cycles.This observation matches the transition between the nucleation and growth regimes in Fig. 8, and supports the hypothesis that the Pt grows faster on the SrTiO 3 (001) substrate.Grazing-incidence small angle X-ray scattering (GISAXS) was utilized to study the evolution in surface morphology with increasing Pt ALD cycles and showed that both the Pt nanoparticle size and inter-particle distance increased linearly with the number of cycles.The surface area of the single crystal SrTiO 3 (001) substrate was far too low to facilitate catalytic testing by conventional methods.However, the surface reactions for Pt ALD should be independent of substrate morphology.Using this assumption, Pt was deposited on high surface area (20 m 2 /g) SrTiO 3 nanocubes with a size of ~ 60 nm that were predominantly terminated with (001) facets.SEM images of the resulting materials revealed monodispersed Pt nanoparticles supported on the SrTiO 3 nanocubes (Fig. 9).During the early stages of Pt ALD on the SrTiO 3 nanocubes the mass was found to increase by 4.4 wt% per cycle, 2x higher than the value predicted using the steady-state growth rate for Pt of ~0.5 Å per cycle 33,31b .Evidently, the enhanced Pt uptake observed during nucleation on the SrTiO 3 s i n g l e c r y s t a l a l s o o c c u r s o n n a n o p h a s e S r T i O 3 , suggesting that the Pt ALD is indeed independent of substrate morphology.X-ray scattering showed that both the Pt nanoparticle size and inter-particle spacing increased linearly with the number of Pt ALD cycles, consistent with the single crystal results and supporting a diffusional processes for nanoparticle formation.Figure 10 shows the size of the ALD Pt nanoparticles as determined from line broadening of the Pt(111) peak using wide angle X-ray scattering measurements.As with Pd, the ALD Pt nanoparticle size could be controlled precisely in the nm regime by adjusting the number of ALD cycles.
The ALD Pt nanoparticles supported on SrTiO 3 nanocubes were significantly more active for propane oxidation than comparable catalysts prepared on a γ-Al 2 O 3 support, emphasizing the important role played by the support 36 .Fig. 10.Pt nanoparticle size on SrTiO 3 nanocubes versus Pt ALD cycles as determined using X-ray diffraction.

In-situ X-ray absorption studies of Pt ALD
A detailed understanding of the surface chemistry for noble metal ALD can lead to better methods for controlling the nanoparticle size, composition, and dispersion.X-ray absorption spectroscopy (XAS), is a powerful tool for determining the local geometric and electronic structure of materials under typical ALD process conditions.Marshall and co-workers used in situ XAS to study Pt ALD over γ-Al

ALD of mixed-noble metal catalysts
Bimetallic catalysts offer the possibility to combine the unique advantages of each component, allowing the catalytic properties to be tuned by adjusting the nanoparticle composition and structure.However, the design and economical synthesis of catalysts at the atomic scale represents a scientific Grand Challenge 35 .ALD offers a potential solution to this challenge.As with the pure Pd and Pt nanoparticles described above, the size of bimetallic particles should be controlled by the total number of ALD cycles performed.Moreover, the composition will be dictated by the relative number of ALD cycles used for each component.Finally, the structure of the bimetallic nanoparticles might be controlled by the order in which the individual cycles are executed.One of the appeals of ALD for the atom scale synthesis of bimetallics is that once a procedure is developed to create the desired nanoparticles, the same process can be used to deposit them on virtually any substrate, and at any quantity.

ALD of iridium-platinum films
To demonstrate the viability of mixed-noble metal ALD, Elam and coworkers synthesized thin-film mixtures of iridium and platinum using iridium (III) acetylacetonate -O 2 cycles for Ir ALD and MeCpPtMe 3 -O 2 cycles for Pt ALD at 300 °C 9 .In situ QCM measurements were performed using various Ir:Pt dosing ratios.These measurements found that the growth rates of Pt and Ir remained constant regardless of the dosing ratio, indicating that both the Ir and Pt ALD proceed equally well on either metal surface.This allowed the composition of the Ir-Pt mixed metal films to be easily controlled using the relative number of Ir cycles, and predicted using a simple rule-of-mixtures formula (Fig. 12).The lattice parameter for the Ir-Pt thin films was determined using X-ray diffraction measurements and was found to vary smoothly between the values of the pure Ir and Pt as the composition was adjusted, consistent with well-mixed, bimetallic alloys.Using this method, conformal Ir-Pt films were deposited successfully on high aspect ratio surfaces, suggesting that coating porous materials using this method should be feasible.

ALD of platinum-ruthenium nanoparticles
Pt-Ru mixed-metal films were prepared using MeCpPtMe

ALD of platinum-palladium nanoparticles
Pt-Pd mixed-metal nanoparticles ~1 nm diameter were synthesized over ALD modified SiO 2 gel with a surface area of 100 m 2 /g using MeCpPtMe 3 -O 2 cycles for Pt ALD and Pd(hfac) 2 -HCOH cycles for Pd ALD.The composition of the Pt-Pd nanoparticles could be adjusted in two ways.Due to the different reaction kinetics for the Pt and Pd ALD processes, the Pt metal loading could be varied by adjusting the deposition temperature while the Pd loading remained constant with temperature.Consequently, the Pt-Pd composition could be controlled through the deposition temperature.In addition, the composition could be tuned using the ratio of Pt to Pd ALD cycles.The scanning transmission electron microscopy (STEM) image in Fig. 14a illustrates the homogeneity of the as-prepared Pt-Pd mixed-metal nanoparticles prepared using a 1:1 molar ratio supported by ALD Al 2 O 3 -coated SiO 2 gel.The mean size of the as-prepared Pt-Pd nanoparticles synthesized using one Pt ALD cycle followed by one Pd ALD cycle was 1.1 ± 0.2 nm.After 3.5% H 2 treatment at 250 °C for one hour, the particle size did change appreciably (Fig. 14b), indicating a high thermal stability for the Pt-Pd nanoparticles.The structure of the ALD Pt-Pd nanoparticles was investigated using XAS measurements at both the Pt L 3 edge (11.56 KeV) and the Pd K edge (24.35 KeV).The as-prepared samples were reduced in H 2 at 250 °C for one hour to obtain a fully metallic state prior to performing the XAS measurements.Small shifts in the edge position and changes in shape for both the Pt and Pd edges were clearly observed.Significant changes in the magnitude and imaginary part of both the Pt and Pd extended X-ray absorption fine structure (EXAFS) measurements indicated second scatterers in the first shell structure, i.e., a bimetallic nanoparticle.Furthermore, EXAFS model fitting showed that Pt-Pd forms a Pt-core, Pd-shell nanostructure, independent of the preparation temperature and ALD pulse sequence.Density functional theory (DFT) was used to calculate the lowest energy configuration for the Pt-Pd binary system.In vacuum, there was no clear preference for either a Pt-or Pd-rich surface.However, the Pd-rich surface was found to be the most stable with one monolayer of hydrogen adsorbed, in good agreement with EXAFS results 37 .

Stabilization of noble metal nanoparticles
The stability of small particles against sintering is a serious problem limiting the application of metal nanoparticles.This problem is particularly severe for supported noble metal catalysts where sintering at high temperatures is a major contributor to catalyst deactivation.38a-d Various methods have been developed to encapsulate noble metal nanoparticles in porous materials using techniques such as chemical vapor deposition, grafting, micro-emulsion, and dendrimer encapsulation to form core-shell structures.39a-h Some of these encapsulated nanoparticles showed good sintering resistance up to 800 °C.However, in nearly all cases the catalytic activity was greatly reduced due to the mass transfer resistance imposed by the protective shell (usually tens of nm thick).In contrast to these previous methods, ALD should enable precise control over the thickness of the protective layer to achieve an optimum balance between enhanced stability and increased mass transfer resistance.To explore this possibility, Al 2 O 3 ALD was used to form protective "over-coats" on ALD Pd nanoparticle catalysts.The catalytic activity and stability of the over-coated catalysts were evaluated using the methanol decomposition reaction.Surprisingly, up to a certain thickness formed using 16 ALD Al 2 O 3 cycles, the protective layers preserved or even slightly enhanced the catalytic activity compared to the same catalyst without Al 2 O 3 overcoating (Fig. 15). 40The reason for this behavior was revealed through infrared spectroscopic measurements of adsorbed CO designed to probe the Pd surface.These measurements showed that the ALD Al 2 O 3 over-coats preferentially nucleate at Pd corners, steps, and edges while leaving the catalytically active Pd (111) facets accessible for methanol conversion.An additional benefit of the over-coating was that the defect sites where the Al 2 O 3 preferentially formed were also responsible for the undesired catalytic reaction to form coke. Consequently, the selectivity of the Pd catalyst for methanol decomposition could be controlled by the site-specific over-coating treatment to preferentially form CO and H 2 versus coke.
In addition to these changes in catalytic behavior, the ALD Al 2 O 3 over-coats virtually eliminated the nanoparticle sintering exhibited by the uncoated Pd catalysts at elevated temperatures.The fact that the Pd surfaces were still accessible to the methanol and the CO probe molecules even after 8 ALD Al 2 O 3 cycles indicates that the ALD Al 2 O 3 over-coats are www.intechopen.comporous.To understand this behavior, the mechanism for Al 2 O 3 ALD on Pd surfaces was investigated by combing in situ QCM and QMS experimental studies with density functional theory (DFT) calculations. 37Both the experimental results and DFT calculations indicated that when TMA reacts on the Pd surface, -CH 3 * surface species are deposited that inhibit further TMA chemisorption.This inhibition likely introduces discontinuities in the Al 2 O 3 film and gives rise to the porosity.The porosity of the ALD Al 2 O 3 overcoats could be increased through high temperature treatment or prolonged reaction at elevated temperatures, suggesting that the Pd catalyst might be modified by tuning the porosity of the Al 2 O 3 over-coats to optimize a particular reaction.

Conclusion
Atomic layer deposition is a powerful method for catalyst synthesis.The self-limiting surface chemistry of ALD provides digital, sub-nm control over the amount of material deposited and allows nanoporous, high surface area materials to be coated uniformly.Noble metal nanoparticles can be prepared by ALD including Pd, Pt, Ir, and Ru, that are highly dispersed and uniform, and the size can be controlled easily on the nm scale by adjusting growth parameters such as the number of ALD cycles.By combining the ALD processes for two different noble metals, bimetallic nanoparticles and films and can be synthesized where the composition is dictated by the relative number of ALD cycles used for the two components.The capability to form uniform, continuous, ultrathin films of metal oxide support materials such as Al 2 O 3 , TiO 2 , and ZrO 2 , as well as size-selected catalytic noble metal nanoparticles, allows a catalyst to be fabricated starting from nearly any convenient template through a sequence of ALD processes.ALD can be used to stabilize noble metal nanoparticles while preserving their catalytic activity by forming porous overcoats that limit agglomeration but still permit access to the metal surface.The scale-up of ALD synthesis is straightforward owing to the self-saturating surface reactions and gas-phase precursors, so that novel materials developed in the lab can be manufactured for industrial use.The application of ALD technology to catalyst synthesis is an active area of research, and new capabilities are certain to emerge in the near future.

Fig. 2 .
Fig. 2. (a) Saturation of ALD Al 2 O 3 growth rate versus TMA exposure; (b) Linear growth of ALD Al 2 O 3 versus number of Al 2 O 3 ALD cycles.

Fig. 4 .
Fig. 4. Nucleation of Pd on Al 2 O 3 using different Pd ALD timing sequences measured by in situ QCM.The timing sequence numbers designate the Pd precursor dose time, Pd precursor purge time, HCOH dose time, and HCOH purge time, respectively, in seconds.7

Fig. 12 .
Fig. 12. Composition of ALD Ir-Pt films versus percentage of Ir ALD cycles measured by quartz crystal microbalance (QCM) and X-ray fluorescence (XRF), and predicted using the rule-of-mixtures (RoM).
3 -O 2 cycles for Pt ALD and 2,4-(dimethylpentadienyl)(ethylcyclopentadienyl) ruthenium (II) (Ru(DER)) -O 2 cycles for Ru ALD at 300°C36 .Similar to the bimetallic Ir-Pt thin films, the growth rates of the Pt and Ru measured by QCM during the Pt-Ru mixed-metal ALD were in close agreement with the growth rates of the pure ALD Pt and Ru.Next, Pt-Ru nanoparticles were synthesized using 2 cycles Ru(DER)/O 2 ; 1 cycle MeCpPtMe 3 /O 2 ; and 1 cycle Ru(DER)/O 2 over spherical Al 2 O 3 nanopowder with a surface area of ~35 m 2 /g yielding an average particle size of 1.2 ± 0.3 nm.Figure13shows the results of XAS measurement performed at the Ru K-edge (22.12 KeV).The Ru K-edge of Ru-Pt nanoparticles is shifted by ~3 eV to higher energy compared to the Ru/SiO 2 standard, suggesting the formation of bimetallic Pt-Ru.Furthermore, the magnitude of the Fourier transform of the Ru K-edge for the Ru-Pt nanoparticles clearly shows different features compared to the Ru nanoparticle standard, indicating the existence of Pt atoms in the first coordination shell of the Ru.Ru K-edge fitting yielded coordination numbers of 3.8 for Ru-Ru and 4.5 for Ru-Pt.These measurements were sufficient to confirm that the nanoparticles were bimetallic, but structure determination (core-shell versus alloy) would require XAS data for the Pt K-edge.The Ru-Pt nanoparticles supported on spherical Al 2 O 3 nanopowder exhibited a much higher reactivity in the methanol decomposition reaction compared to a physical mixture of Ru and Pt monometallic catalysts, consistent with the unique atomic arrangement of a bimetallic catalyst.

Fig. 13 .
Fig. 13.XAS measurements showing (a) Ru K-edge for ALD Ru-Pt/Al 2 O 3 and a reference 3% Ru/SiO 2 ; (b) Fourier transforms of the absorption spectra where the solid lines show the magnitude and the broken lines shows the imaginary part.

Fig. 15 .
Fig. 15.Methanol conversion for Pd catalysts with 0 to 32 cycles of ALD Al 2 O 3 over-coating in the methanol decomposition reaction carried out at 250 and 270 °C.40 To prepare Pt nanoparticles on high surface area supports, longer dose and purge times of several minutes are needed to allow complete saturation and precursor removal.Similar to Pd, Pt ALD on oxide surfaces can be divided into two regimes: nucleation and growth.The growth regime is characterized by a constant growth per cycle because the surface reactions have achieved a steady state.The mechanism for Pt ALD in the steady-state growth regime has been well studied and is given by 31 : * + 24 O 2  2 Pt* +3 O* + 16 CO 2 + 13 H 2 O